# A Cosserat crystal plasticity and phase field theory for ... Cosserat crystal plasticity and phase...

date post

05-May-2018Category

## Documents

view

213download

0

Embed Size (px)

### Transcript of A Cosserat crystal plasticity and phase field theory for ... Cosserat crystal plasticity and phase...

HAL Id: hal-01615967https://hal.archives-ouvertes.fr/hal-01615967

Submitted on 12 Oct 2017

HAL is a multi-disciplinary open accessarchive for the deposit and dissemination of sci-entific research documents, whether they are pub-lished or not. The documents may come fromteaching and research institutions in France orabroad, or from public or private research centers.

Larchive ouverte pluridisciplinaire HAL, estdestine au dpt et la diffusion de documentsscientifiques de niveau recherche, publis ou non,manant des tablissements denseignement et derecherche franais ou trangers, des laboratoirespublics ou privs.

A Cosserat crystal plasticity and phase field theory forgrain boundary migration

Anna Ask, Samuel Forest, Benoit Appolaire, Kais Ammar, Oguz UmutSalman

To cite this version:Anna Ask, Samuel Forest, Benoit Appolaire, Kais Ammar, Oguz Umut Salman. A Cosserat crystalplasticity and phase field theory for grain boundary migration. 2017.

https://hal.archives-ouvertes.fr/hal-01615967https://hal.archives-ouvertes.fr

A Cosserat crystal plasticity and phase field theory for grain boundarymigration

Anna Aska, Samuel Foresta,, Benoit Appolaireb, Kais Ammara, Oguz Umut Salmanc

aMINES ParisTech, PSL Research University, MAT Centre des materiaux,CNRS UMR 7633, BP 87 91003 Evry, France5

bLEM, CNRS/ONERA, BP 72, 92322 Chatillon Cedex, FrancecCNRS, LSPM UPR3407, Universite Paris 13, Sorbonne Paris Cite, 93430, Villetaneuse, France

Abstract

The microstructure evolution due to thermomechanical treatment of metals can largely be described by

viscoplastic deformation, nucleation and grain growth. These processes take place over different length

and time scales which present significant challenges when formulating simulation models. In particular,

no overall unified field framework exists to model concurrent viscoplastic deformation and recrystal-

lization and grain growth in metal polycrystals. In this work a thermodynamically consistent diffuse

interface framework incorporating crystal viscoplasticity and grain boundary migration is elaborated.

The KobayashiWarrenCarter (KWC) phase field model is extended to incorporate the full mechanical

coupling with material and lattice rotations and evolution of dislocation densities. The Cosserat crystal

plasticity theory is shown to be the appropriate framework to formulate the coupling between phase field

and mechanics with proper distinction between bulk and grain boundary behaviour.

Keywords: Cosserat crystal plasticity, Phase field method, Dynamic recrystallization

1. Introduction10

1.1. Scope of the work

The microstructure of a polycrystalline metallic material is characterized by the shape and distribution

of differently oriented grains. Macroscopic material properties such as strength and ductility can be tuned

by thermomechanical processing which significantly alters the microstructure of the metal at the grain

scale through viscoplastic deformation and subsequent (sequential) or concurrent (dynamic) nucleation15

and growth of new grains. To date, the deformation, nucleation and grain growth tend to be treated using

a combination of different methods, even in coupled approaches. Regardless of the choice of method, it is

important to identify the variables which are sufficient to describe the microstructure and its evolution.

Nucleation tends to be favored at sites of large misorientation or lattice curvature and the mobility of

Corresponding authorEmail address: samuel.forest@ensmp.fr (Samuel Forest)

Preprint submitted to Elsevier October 9, 2017

migrating grains is also closely related to the misorientation (Humphreys and Hatherly, 2004; Sutton20

and Ballufi, 2007; Gottstein and Shvindlerman, 2010). On the one hand, viscoplastic deformation may

result in significant reorientation of the crystal lattice and the development of heterogeneous orientation

distributions within previously uniformly oriented grains. On the other hand, a migrating grain boundary

will also result in reorientation since the grain orientation of material points in the region it passes will

change from that of the old to that of the growing grain. In order to obtain a strongly coupled scheme25

suitable to model concurrent viscoplastic deformation and grain growth, it is necessary to consider the

evolution of the grain orientation during these respective processes. Plastic deformation also leads to

build-up of dislocations inside the grains. The resulting dislocation densities tend not to be homogeneous

and nucleation is favored at sites with a high dislocation content. Furthermore, stored energy due to

dislocations is an important driving force for grain boundary migration.30

Crystal plasticity models provide the most complete tools to model microstructure evolution at the

grain scale induced by viscoplastic deformation, including heterogeneous reorientation and dislocation

density build-up (Cailletaud et al., 2003; Roters et al., 2010). For the nucleation and growth of new

grains, it is common to combine some criterion for the generation of new nuclei with a model for migrating

grain boundaries. The tracking of the moving interface can be done explicitly or implicitly. Examples35

of the latter are level-set (Chen, 1995; Bernacki et al., 2008) and phase-field methods. In the literature,

there are two main phase field approaches used to model grain growth in solid polycrystals: multi-phase

field methods as introduced by Steinbach et al. (1996); Steinbach and Pezzolla (1999) or Fan and Chen

(1997) and orientation field based models of the type introduced by Kobayashi et al. (2000); Warren

et al. (2003). In particular, by using the formalism of generalized forces introduced by Gurtin (1996);40

Gurtin and Lusk (1999), the phase field methods can be derived from the same energy principles as the

governing equations of mechanics, making them a strong candidate for a coupled theory.

1.2. Phase-field models for GB migration

To model grain growth using a multi-phase field model, each of N non-conserved phase field variables

i, i = 1, . . . , N ;Ni i = 1 is associated with a grain orientation. Note that in the multi-phase approach,45

the phase fields themselves are not the crystal orientations (even if they are referred to as orientation

fields in e.g. Fan and Chen (1997)) but rather represent the fraction of phase i, of a given orientation,

present at a material point. Inside a grain, only one phase field variable takes the value 1 and all the

others are zero. Steinbach et al. (1996) suggested that all possible orientations be divided into N = 10

classes according to a Potts model. More generally, any discrete number of possible orientations may50

be used but of course, the problem size will grow with N . Fan and Chen (1997) studied the influence

2

of the number of orientations on the grain growth simulations, demonstrating that in their proposed

model, with few allowed orientations the tendency was that grains of equal orientation coalesced whereas

with a larger number of allowed orientations, grain boundary migration was favored. One attractive

feature of the multi-phase field approach is that the model parameters can easily be associated with55

the measurable quantities mobility, grain boundary energy and interface thickness. The inclusion of

misorientation dependency and anisotropy is likewise straightforward (Steinbach et al., 1996). However,

the multi-phase field model is not suitable for a strongly coupled approach based on lattice orientation

since it does not contain an equation that allows for evolution of the orientation within a grain. The

orientation of a material point can only change due to grain boundary migration. This is not compatible60

with heterogeneous lattice rotation developing in a grain due to plastic deformation. Since each phase

is associated with a single orientation, new phase fields must be added to the model to accommodate

each incremental change in orientation due to e.g. viscoplastic deformation. Even then, only a discrete

number of orientations can be modeled. In reality, all possible crystal orientations should be considered.

The orientation phase field model due to Kobayashi et al. (2000); Warren et al. (2003) (often and65

in what follows denoted the KWC model) requires only two fields. One is an order parameter

[0, 1] which can be regarded as a measure of crystalline order called crystallinity. In a solidification

model = 0 would correspond to the liquid phase and = 1 to the solid phase. For grains in a

polycrystal the variation of enables a distinction between the bulk of the grain and the grain boundary,

being minimal inside diffuse graind boundaries. The other phase field parameter is the orientation70

field , which in the KWC two-dimensional formulation denotes the orientation of the crystal lattice

with respect to the laboratory frame. It is less straightforward to associate the parameters of the KWC

model with measurable quantities compared to the multi-phase model. Lobkovsky and Warren (2001)

found the sharp interface limit of the KWC model through formal asymptotics, providing expressions

for the grain boundary energy and mobility which enables parameter calibration based on comparisons75

with experimental data. While originally formulated in two dimensions, extensions to three dimensional

orientation field based formulations are discussed in e.g. Kobayashi and Warren (200

*View more*